Download presentation

Presentation is loading. Please wait.

Published byAutumn Hinsley Modified about 1 year ago

1
ISSUES TO ADDRESS... Historical retrospective Henry Bragg Equation XRD-analysis How to read XRD patterns? Exclusions What questions can be answered by XRD method? X-Ray Diffraction (XRD) CHAPTER 3: CRYSTAL STRUCTURES X-Ray Diffraction (XRD)

2
Scale of Structure Organization

3
Sir William Henry Bragg Sir William Henry Bragg: William Henry and William Lawrence Bragg (father and son) found a simple interpretation of von Laue’s experiment. They assume that each crystal plane reflects radiation as a mirror and analyze this situation for cases of constructive and destructive interference. The most important thing in science is not so much to obtain new facts as to discover new ways of thinking about them. Conditions for reflection: Noble prize 1915! Bragg’s law

4
Derivation of Bragg’s law Path difference Δ= 2x => phase shift Constructive interference if Δ=nλ This gives the criterion for constructive interference: θ θ θ x d hkl Bragg’s law tells you at which angle θ B to expect maximum diffracted intensity for a particular family of crystal planes. For large crystals, all other angles give zero intensity.

5
The powder diffractometers typically use the Bragg-Brentano geometry The incident angle, , is defined between the X-ray source and the sample. The diffracted angle, 2 , is defined between the incident beam and the detector angle. The incident angle is always ½ of the detector angle 2 . In a :2 instrument (e.g. Rigaku RU300), the tube is fixed, the sample rotates at °/min and the detector rotates at 2 °/min. In a : instrument (e.g. PANalytical X’Pert Pro), the sample is fixed and the tube rotates at a rate - °/min and the detector rotates at a rate of °/min. X-ray tube Detector

6
A single crystal specimen in a Bragg-Brentano diffractometer would produce only one family of peaks in the diffraction pattern. 22 At 20.6 °2 , Bragg’s law fulfilled for the (100) planes, producing a diffraction peak. The (110) planes would diffract at 29.3 °2 ; however, they are not properly aligned to produce a diffraction peak (the perpendicular to those planes does not bisect the incident and diffracted beams). Only background is observed. The (200) planes are parallel to the (100) planes. Therefore, they also diffract for this crystal. Since d 200 is ½ d 100, they appear at 42 °2 .

7
A polycrystalline sample should contain thousands of crystallites. Therefore, all possible diffraction peaks should be observed. 22 22 22 For every set of planes, there will be a small percentage of crystallites that are properly oriented to diffract (the plane perpendicular bisects the incident and diffracted beams). Basic assumptions of powder diffraction are that for every set of planes there is an equal number of crystallites that will diffract and that there is a statistically relevant number of crystallites, not just one or two.

8
Example: Diffraction Patterns Each peak represents the solution to Bragg’s law for known radiation wavelength ( = 0.154nm) The unique relationship between such patterns and crystal structures provide a powerful tool for identification of the phase composition of powders and polycrystalline materials.

9

10

11
Basis and Bravais Structure Factor Terms The following simple table giving the integer values of F BR for the different types of centering translations. Keep in mind that these are valid for any crystal system.

12

13

14

15
Summary

Similar presentations

© 2016 SlidePlayer.com Inc.

All rights reserved.

Ads by Google